Preparation and Characterization of {[M(dmb)2]TCNQ.xTCNQ° }n Polymers (M = Cu,Ag; dmb = 1,8-Diisocyano-p-menthane; x = 0, 0.5, 1.0, 1.5; TCNQ = 7,7,8,8-Tetracyano-p-quinodimethane) and Design of New Semi- and Photoconducting Organometallic Materials
Daniel Fortin; Marc Drouin; Pierre D. Harvey; Inorganic Chemistry 39 (2000) 2758–2769; doi:10.1021/ic990975o

data_4321089
_publ_section_title
;
 Preparation and Characterization of {[M(dmb)2]TCNQ.xTCNQ\% }n Polymers (M
 = Cu,Ag; dmb = 1,8-Diisocyano-p-menthane; x = 0, 0.5, 1.0, 1.5; TCNQ =
 7,7,8,8-Tetracyano-p-quinodimethane) and Design of New Semi- and
 Photoconducting Organometallic Materials
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2758
_journal_page_last               2769
_journal_paper_doi               10.1021/ic990975o
_journal_volume                  39
_journal_year                    2000
_chemical_formula_sum            'C70 H80 Ag2 N14 O2'
_chemical_formula_weight         1365.22
_chemical_name_systematic
;
Ag(dmb)2 DCTC
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 112.12(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   26.273(3)
_cell_length_b                   9.730(3)
_cell_length_c                   31.526(3)
_cell_measurement_temperature    293(2)
_cell_volume                     7466(3)
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuKa
_diffrn_radiation_wavelength     1.54060
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.1530
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            4535
_diffrn_reflns_theta_full        40.00
_diffrn_reflns_theta_max         40.00
_diffrn_reflns_theta_min         1.51
_exptl_absorpt_coefficient_mu    4.596
_exptl_crystal_density_diffrn    1.215
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2832
_refine_diff_density_max         1.900
_refine_diff_density_min         -0.973
_refine_diff_density_rms         0.164
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.473
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     364
_refine_ls_number_reflns         4535
_refine_ls_number_restraints     92
_refine_ls_restrained_S_all      1.462
_refine_ls_R_factor_all          0.2301
_refine_ls_R_factor_gt           0.1346
_refine_ls_shift/su_max          0.021
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1000P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2999
_refine_ls_wR_factor_ref         0.3243
_reflns_number_gt                2194
_reflns_number_total             4535
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic990975o_4.cif
_cod_data_source_block           4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_database_code               4321089